General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 7.9 - 7.93 g/cm³ Show Material materials with Density of 7.9 - 7.93 g/cm³ |

Mechanical

Property | Temperature | Value |
---|---|---|

Elastic modulus | -100.0 °C | 206 GPa Show Material materials with Elastic modulus of 206 GPa |

20.0 °C | 196 - 200 GPa Show Material materials with Elastic modulus of 196 - 200 GPa | |

95.0 °C | 194.43 GPa Show Material materials with Elastic modulus of 194.43 GPa | |

100.0 °C | 190 - 194 GPa Show Material materials with Elastic modulus of 190 - 194 GPa | |

150.0 °C | 189.61 GPa Show Material materials with Elastic modulus of 189.61 GPa | |

200.0 °C | 182 - 186 GPa Show Material materials with Elastic modulus of 182 - 186 GPa | |

205.0 °C | 184.78 GPa Show Material materials with Elastic modulus of 184.78 GPa | |

260.0 °C | 179.95 GPa Show Material materials with Elastic modulus of 179.95 GPa | |

300.0 °C | 174 - 179 GPa Show Material materials with Elastic modulus of 174 - 179 GPa | |

315.0 °C | 175.13 GPa Show Material materials with Elastic modulus of 175.13 GPa | |

370.0 °C | 170.99 GPa Show Material materials with Elastic modulus of 170.99 GPa | |

400.0 °C | 166 - 172 GPa Show Material materials with Elastic modulus of 166 - 172 GPa | |

425.0 °C | 166.16 GPa Show Material materials with Elastic modulus of 166.16 GPa | |

485.0 °C | 161.34 GPa Show Material materials with Elastic modulus of 161.34 GPa | |

500.0 °C | 158 - 165 GPa Show Material materials with Elastic modulus of 158 - 165 GPa | |

540.0 °C | 157.2 GPa Show Material materials with Elastic modulus of 157.2 GPa | |

595.0 °C | 151.69 GPa Show Material materials with Elastic modulus of 151.69 GPa | |

600.0 °C | 150 GPa Show Material materials with Elastic modulus of 150 GPa | |

650.0 °C | 147.54 GPa Show Material materials with Elastic modulus of 147.54 GPa | |

700.0 °C | 142 GPa Show Material materials with Elastic modulus of 142 GPa | |

705.0 °C | 142.72 GPa Show Material materials with Elastic modulus of 142.72 GPa | |

760.0 °C | 137.9 GPa Show Material materials with Elastic modulus of 137.9 GPa | |

800.0 °C | 134 GPa Show Material materials with Elastic modulus of 134 GPa | |

815.0 °C | 133.76 GPa Show Material materials with Elastic modulus of 133.76 GPa | |

870.0 °C | 128.93 GPa Show Material materials with Elastic modulus of 128.93 GPa | |

900.0 °C | 127 GPa Show Material materials with Elastic modulus of 127 GPa | |

1000.0 °C | 120 GPa Show Material materials with Elastic modulus of 120 GPa | |

Elongation | 20.0 °C | 40 % Show Material materials with Elongation of 40 % |

Elongation, transverse | 20.0 °C | 30 % Show Material materials with Elongation, transverse of 30 % |

Hardness, Brinell | 20.0 °C | 230 [-] Show Material materials with Hardness, Brinell of 230 [-] |

Hardness, Brinell, trans | 20.0 °C | 230 [-] Show Material materials with Hardness, Brinell, trans of 230 [-] |

Poisson's ratio | 20.0 °C | 0.27 [-] Show Material materials with Poisson's ratio of 0.27 [-] |

95.0 °C | 0.28 [-] Show Material materials with Poisson's ratio of 0.28 [-] | |

150.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

205.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

260.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

315.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

370.0 °C | 0.31 [-] Show Material materials with Poisson's ratio of 0.31 [-] | |

425.0 °C | 0.31 [-] Show Material materials with Poisson's ratio of 0.31 [-] | |

485.0 °C | 0.32 [-] Show Material materials with Poisson's ratio of 0.32 [-] | |

540.0 °C | 0.33 [-] Show Material materials with Poisson's ratio of 0.33 [-] | |

595.0 °C | 0.33 [-] Show Material materials with Poisson's ratio of 0.33 [-] | |

650.0 °C | 0.32 [-] Show Material materials with Poisson's ratio of 0.32 [-] | |

705.0 °C | 0.33 [-] Show Material materials with Poisson's ratio of 0.33 [-] | |

760.0 °C | 0.35 [-] Show Material materials with Poisson's ratio of 0.35 [-] | |

815.0 °C | 0.35 [-] Show Material materials with Poisson's ratio of 0.35 [-] | |

870.0 °C | 0.36 [-] Show Material materials with Poisson's ratio of 0.36 [-] | |

Unlock all property charts | ||

Shear modulus | 20.0 °C | 78.6 GPa Show Material materials with Shear modulus of 78.6 GPa |

95.0 °C | 75.84 GPa Show Material materials with Shear modulus of 75.84 GPa | |

150.0 °C | 73.77 GPa Show Material materials with Shear modulus of 73.77 GPa | |

205.0 °C | 71.71 GPa Show Material materials with Shear modulus of 71.71 GPa | |

260.0 °C | 69.64 GPa Show Material materials with Shear modulus of 69.64 GPa | |

315.0 °C | 67.57 GPa Show Material materials with Shear modulus of 67.57 GPa | |

370.0 °C | 65.5 GPa Show Material materials with Shear modulus of 65.5 GPa | |

425.0 °C | 63.43 GPa Show Material materials with Shear modulus of 63.43 GPa | |

485.0 °C | 61.36 GPa Show Material materials with Shear modulus of 61.36 GPa | |

540.0 °C | 59.3 GPa Show Material materials with Shear modulus of 59.3 GPa | |

595.0 °C | 57.23 GPa Show Material materials with Shear modulus of 57.23 GPa | |

650.0 °C | 55.85 GPa Show Material materials with Shear modulus of 55.85 GPa | |

705.0 °C | 53.78 GPa Show Material materials with Shear modulus of 53.78 GPa | |

760.0 °C | 51.11 GPa Show Material materials with Shear modulus of 51.11 GPa | |

815.0 °C | 49.64 GPa Show Material materials with Shear modulus of 49.64 GPa | |

870.0 °C | 47.57 GPa Show Material materials with Shear modulus of 47.57 GPa | |

Unlock all property charts | ||

Tensile strength | 20.0 °C | 510 - 740 MPa Show Material materials with Tensile strength of 510 - 740 MPa |

100.0 °C | 435 MPa Show Material materials with Tensile strength of 435 MPa | |

150.0 °C | 400 MPa Show Material materials with Tensile strength of 400 MPa | |

200.0 °C | 370 MPa Show Material materials with Tensile strength of 370 MPa | |

250.0 °C | 350 MPa Show Material materials with Tensile strength of 350 MPa | |

300.0 °C | 340 MPa Show Material materials with Tensile strength of 340 MPa | |

350.0 °C | 335 MPa Show Material materials with Tensile strength of 335 MPa | |

400.0 °C | 330 MPa Show Material materials with Tensile strength of 330 MPa | |

450.0 °C | 320 MPa Show Material materials with Tensile strength of 320 MPa | |

500.0 °C | 310 MPa Show Material materials with Tensile strength of 310 MPa | |

550.0 °C | 300 MPa Show Material materials with Tensile strength of 300 MPa | |

Unlock all property charts | ||

Tensile strength, transverse | 20.0 °C | 510 - 740 MPa Show Material materials with Tensile strength, transverse of 510 - 740 MPa |

Yield strength Rp0.2 | 20.0 °C | 205 MPa Show Material materials with Yield strength Rp0.2 of 205 MPa |

100.0 °C | 175 MPa Show Material materials with Yield strength Rp0.2 of 175 MPa | |

150.0 °C | 165 MPa Show Material materials with Yield strength Rp0.2 of 165 MPa | |

200.0 °C | 155 MPa Show Material materials with Yield strength Rp0.2 of 155 MPa | |

250.0 °C | 145 - 147 MPa Show Material materials with Yield strength Rp0.2 of 145 - 147 MPa | |

300.0 °C | 136 MPa Show Material materials with Yield strength Rp0.2 of 136 MPa | |

350.0 °C | 130 MPa Show Material materials with Yield strength Rp0.2 of 130 MPa | |

400.0 °C | 125 MPa Show Material materials with Yield strength Rp0.2 of 125 MPa | |

450.0 °C | 121 MPa Show Material materials with Yield strength Rp0.2 of 121 MPa | |

500.0 °C | 119 MPa Show Material materials with Yield strength Rp0.2 of 119 MPa | |

550.0 °C | 118 MPa Show Material materials with Yield strength Rp0.2 of 118 MPa | |

Unlock all property charts | ||

Yield strength Rp0.2, transverse | 20.0 °C | 205 MPa Show Material materials with Yield strength Rp0.2, transverse of 205 MPa |

Yield strength Rp1.0 | 20.0 °C | 240 MPa Show Material materials with Yield strength Rp1.0 of 240 MPa |

100.0 °C | 210 MPa Show Material materials with Yield strength Rp1.0 of 210 MPa | |

150.0 °C | 195 MPa Show Material materials with Yield strength Rp1.0 of 195 MPa | |

200.0 °C | 185 MPa Show Material materials with Yield strength Rp1.0 of 185 MPa | |

250.0 °C | 175 MPa Show Material materials with Yield strength Rp1.0 of 175 MPa | |

300.0 °C | 167 MPa Show Material materials with Yield strength Rp1.0 of 167 MPa | |

350.0 °C | 161 MPa Show Material materials with Yield strength Rp1.0 of 161 MPa | |

400.0 °C | 156 MPa Show Material materials with Yield strength Rp1.0 of 156 MPa | |

450.0 °C | 152 MPa Show Material materials with Yield strength Rp1.0 of 152 MPa | |

500.0 °C | 149 MPa Show Material materials with Yield strength Rp1.0 of 149 MPa | |

550.0 °C | 147 MPa Show Material materials with Yield strength Rp1.0 of 147 MPa | |

Unlock all property charts | ||

Yield strength Rp1.0, transverse | 20.0 °C | 240 MPa Show Material materials with Yield strength Rp1.0, transverse of 240 MPa |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | -100.0 °C | 1.49E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.49E-5 1/K | |

20.0 °C | 1.61E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.61E-5 1/K | ||

100.0 °C | 1.6E-5 - 1.67E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.6E-5 - 1.67E-5 1/K | ||

200.0 °C | 1.65E-5 - 1.72E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.65E-5 - 1.72E-5 1/K | ||

300.0 °C | 1.7E-5 - 1.77E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.7E-5 - 1.77E-5 1/K | ||

400.0 °C | 1.75E-5 - 1.81E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.75E-5 - 1.81E-5 1/K | ||

425.0 °C | 1.76E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.76E-5 1/K | ||

485.0 °C | 1.78E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.78E-5 1/K | ||

500.0 °C | 1.8E-5 - 1.84E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.8E-5 - 1.84E-5 1/K | ||

540.0 °C | 1.8E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.8E-5 1/K | ||

595.0 °C | 1.83E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.83E-5 1/K | ||

600.0 °C | 1.88E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.88E-5 1/K | ||

650.0 °C | 1.85E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.85E-5 1/K | ||

700.0 °C | 1.91E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.91E-5 1/K | ||

705.0 °C | 1.87E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.87E-5 1/K | ||

800.0 °C | 1.94E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.94E-5 1/K | ||

900.0 °C | 1.97E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.97E-5 1/K | ||

1000.0 °C | 2E-5 1/K Show Material materials with Coefficient of thermal expansion of 2E-5 1/K | ||

Unlock all property charts | |||

Melting point | 1230 - 1480 °C Show Material materials with Melting point of 1230 - 1480 °C | Typical for Austenitic Stainless Steel | |

Specific heat capacity | -100.0 °C | 440 J/(kg·K) Show Material materials with Specific heat capacity of 440 J/(kg·K) | |

20.0 °C | 472 - 500 J/(kg·K) Show Material materials with Specific heat capacity of 472 - 500 J/(kg·K) | ||

100.0 °C | 487 J/(kg·K) Show Material materials with Specific heat capacity of 487 J/(kg·K) | ||

200.0 °C | 503 J/(kg·K) Show Material materials with Specific heat capacity of 503 J/(kg·K) | ||

300.0 °C | 512 J/(kg·K) Show Material materials with Specific heat capacity of 512 J/(kg·K) | ||

400.0 °C | 520 J/(kg·K) Show Material materials with Specific heat capacity of 520 J/(kg·K) | ||

500.0 °C | 530 J/(kg·K) Show Material materials with Specific heat capacity of 530 J/(kg·K) | ||

600.0 °C | 541 J/(kg·K) Show Material materials with Specific heat capacity of 541 J/(kg·K) | ||

700.0 °C | 551 J/(kg·K) Show Material materials with Specific heat capacity of 551 J/(kg·K) | ||

800.0 °C | 559 J/(kg·K) Show Material materials with Specific heat capacity of 559 J/(kg·K) | ||

900.0 °C | 565 J/(kg·K) Show Material materials with Specific heat capacity of 565 J/(kg·K) | ||

1000.0 °C | 571 J/(kg·K) Show Material materials with Specific heat capacity of 571 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | 20.0 °C | 14.3 - 15 W/(m·K) Show Material materials with Thermal conductivity of 14.3 - 15 W/(m·K) | |

100.0 °C | 15.8 W/(m·K) Show Material materials with Thermal conductivity of 15.8 W/(m·K) | ||

200.0 °C | 17.5 W/(m·K) Show Material materials with Thermal conductivity of 17.5 W/(m·K) | ||

300.0 °C | 19 W/(m·K) Show Material materials with Thermal conductivity of 19 W/(m·K) | ||

400.0 °C | 20.5 W/(m·K) Show Material materials with Thermal conductivity of 20.5 W/(m·K) | ||

500.0 °C | 21.9 W/(m·K) Show Material materials with Thermal conductivity of 21.9 W/(m·K) | ||

600.0 °C | 23.3 W/(m·K) Show Material materials with Thermal conductivity of 23.3 W/(m·K) | ||

700.0 °C | 24.6 W/(m·K) Show Material materials with Thermal conductivity of 24.6 W/(m·K) | ||

800.0 °C | 26 W/(m·K) Show Material materials with Thermal conductivity of 26 W/(m·K) | ||

900.0 °C | 27.4 W/(m·K) Show Material materials with Thermal conductivity of 27.4 W/(m·K) | ||

1000.0 °C | 28.8 W/(m·K) Show Material materials with Thermal conductivity of 28.8 W/(m·K) | ||

Unlock all property charts | |||

Thermal diffusivity | 20.0 °C | 3.8 mm²/s Show Material materials with Thermal diffusivity of 3.8 mm²/s | |

100.0 °C | 4 mm²/s Show Material materials with Thermal diffusivity of 4 mm²/s | ||

200.0 °C | 4.2 mm²/s Show Material materials with Thermal diffusivity of 4.2 mm²/s | ||

300.0 °C | 4.6 mm²/s Show Material materials with Thermal diffusivity of 4.6 mm²/s | ||

400.0 °C | 4.8 mm²/s Show Material materials with Thermal diffusivity of 4.8 mm²/s | ||

500.0 °C | 4.9 mm²/s Show Material materials with Thermal diffusivity of 4.9 mm²/s | ||

600.0 °C | 5 mm²/s Show Material materials with Thermal diffusivity of 5 mm²/s | ||

700.0 °C | 5.3 mm²/s Show Material materials with Thermal diffusivity of 5.3 mm²/s | ||

800.0 °C | 5.6 mm²/s Show Material materials with Thermal diffusivity of 5.6 mm²/s | ||

900.0 °C | 5.9 mm²/s Show Material materials with Thermal diffusivity of 5.9 mm²/s | ||

1000.0 °C | 6 mm²/s Show Material materials with Thermal diffusivity of 6 mm²/s | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 7.1E-7 - 7.3E-7 Ω·m Show Material materials with Electrical resistivity of 7.1E-7 - 7.3E-7 Ω·m |

100.0 °C | 7.76E-7 Ω·m Show Material materials with Electrical resistivity of 7.76E-7 Ω·m | |

200.0 °C | 8.49E-7 Ω·m Show Material materials with Electrical resistivity of 8.49E-7 Ω·m | |

300.0 °C | 9.14E-7 Ω·m Show Material materials with Electrical resistivity of 9.14E-7 Ω·m | |

400.0 °C | 9.71E-7 Ω·m Show Material materials with Electrical resistivity of 9.71E-7 Ω·m | |

500.0 °C | 1.02E-6 Ω·m Show Material materials with Electrical resistivity of 1.02E-6 Ω·m | |

600.0 °C | 1.07E-6 Ω·m Show Material materials with Electrical resistivity of 1.07E-6 Ω·m | |

700.0 °C | 1.1E-6 Ω·m Show Material materials with Electrical resistivity of 1.1E-6 Ω·m | |

800.0 °C | 1.14E-6 Ω·m Show Material materials with Electrical resistivity of 1.14E-6 Ω·m | |

900.0 °C | 1.17E-6 Ω·m Show Material materials with Electrical resistivity of 1.17E-6 Ω·m | |

1000.0 °C | 1.19E-6 Ω·m Show Material materials with Electrical resistivity of 1.19E-6 Ω·m | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Carbon | 0.08 % Show Material materials with Carbon of 0.08 % |

Chromium | 17 - 19 % Show Material materials with Chromium of 17 - 19 % |

Manganese | 2 % Show Material materials with Manganese of 2 % |

Nickel | 9 - 12 % Show Material materials with Nickel of 9 - 12 % |

Niobium | 1 % Show Material materials with Niobium of 1 % |

Phosphorus | 0.05 % Show Material materials with Phosphorus of 0.05 % |

Silicon | 1 % Show Material materials with Silicon of 1 % |

Sulfur | 0.015 % Show Material materials with Sulfur of 0.015 % |